On October 23rd, 2014, we updated our
By continuing to use LinkedIn’s SlideShare service, you agree to the revised terms, so please take a few minutes to review them.
A 334/A 334M – 04a TABLE 1 Chemical Requirements Element Composition, % A A Grade 1 Grade 3 Grade 6 Grade 7 Grade 8 Grade 9 Grade 11Carbon, max 0.30 0.19 0.30 0.19 0.13 0.20 0.10Manganese 0.40–1.06 0.31–0.64 0.29–1.06 0.90 max 0.90 max 0.40–1.06 0.60 maxPhosphorus, max 0.025 0.025 0.025 0.025 0.025 0.025 0.025Sulfur, max 0.025 0.025 0.025 0.025 0.025 0.025 0.025Silicon ... 0.18–0.37 0.10 min 0.13–0.32 0.13–0.32 ... 0.35 maxNickel ... 3.18–3.82 ... 2.03–2.57 8.40–9.60 1.60–2.24 35.0–37.0Chromium ... ... ... ... ... ... 0.50 maxCopper ... ... ... ... ... 0.75–1.25 ...Cobalt ... ... ... ... ... ... 0.50 maxMolybdenum ... ... ... ... ... ... 0.50 max A For each reduction of 0.01 % carbon below 0.30 %, an increase of 0.05 % manganese above 1.06 % will be permitted to a maximum of 1.35 % manganese.°C] and cool in a controlled atmosphere furnace from an initial 8. Product Analysistemperature of not less than 1550 °F [845 °C]. 8.1 An analysis of either one billet or one length of 6.1.4 Treat as in 6.1.3 and, at the discretion of the manu- ﬂat-rolled stock or one tube shall be made for each heat. Thefacturer, reheat to a suitable tempering temperature. chemical composition thus determined shall conform to the 6.2 Grade 8 tubes shall be heat treated by the manufacturer requirements speciﬁed.by either of the following methods. 8.2 If the original test for product analysis fails, retests of 6.2.1 Quenched and Tempered—Heat to a uniform tempera- two additional billets, lengths of ﬂat-rolled stock, or tubes shallture of 1475 6 25 °F [800 6 15 °C]; hold at this temperature be made. Both retests, for the elements in question, shall meetfor a minimum time in the ratio of 1 h/in. [2 min/mm] of the requirements of the speciﬁcation; otherwise all remainingthickness, but in no case less than 15 min; quench by material in the heat or lot shall be rejected or, at the option ofimmersion in circulating water. Reheat until the pipe attains a the manufacturer, each billet, length of ﬂat-rolled stock, or tubeuniform temperature within the range from 1050 to 1125 °F may be individually tested for acceptance. Billets, lengths of[565 to 605 °C]; hold at this temperature for a minimum time ﬂat-rolled stock, or tubes which do not meet the requirementsin the ratio of 1 h/in. [2 min/mm] of thickness, but in no case of the speciﬁcation shall be rejected.less than 15 min; cool in air or water quench at a rate no lessthan 300 °F [165 °C]/h. 9. Sampling 6.2.2 Double Normalized and Tempered— Heat to a uni- 9.1 For ﬂattening, ﬂare, and ﬂange requirements, the termform temperature of 1650 6 25 °F [900 6 15 °C]; hold at this lot applies to all tubes prior to cutting of the same nominal sizetemperature for a minimum time in the ratio of 1 h/in. [2 and wall thickness which are produced from the same heat ofmin/mm] of thickness, but in no case less than 15 min; cool in steel. When ﬁnal heat treatment is in a batch-type furnace, a lotair. Reheat until the pipe attains a uniform temperature of 1450 shall include only those tubes of the same size and from the6 25 °F [790 6 15 °C]; hold at this temperature for a same heat which are heat treated in the same furnace charge.minimum time in the ratio of 1 h/in. [2 min/mm] of thickness, When the ﬁnal heat treatment is in a continuous furnace, thebut in no case less than 15 min; cool in air. Reheat to a uniform number of tubes of the same size and from the same heat in atemperature within the range from 1050 to 1125 °F [565 to 605 lot shall be determined from the size of the tubes as prescribed°C]; hold at this temperature for a minimum time of 1 h/in. [2 in Table 2.min/mm] of thickness but in no case less than 15 min; cool in 9.2 For tensile and hardness test requirements, the term lotair or water quench at a rate not less than 300 °F [165 °C]/h. applies to all tubes prior to cutting, of the same nominal 6.3 Material from which impact specimens are obtained diameter and wall thickness which are produced from the sameshall be in the same condition of heat treatment as the ﬁnished heat of steel. When ﬁnal heat treatment is in a batch-typetubes. furnace, a lot shall include only those tubes of the same size 6.4 Whether to anneal Grade 11 tubes is per agreement and the same heat which are heat treated in the same furnacebetween purchaser and supplier. When Grade 11 tubes are charge. When the ﬁnal heat treatment is in a continuousannealed they shall be normalized in the range of 1400 to 1600°F [760 to 870 °C]. TABLE 2 Heat-Treatment Lot7. Chemical Composition Size of Tube Size of Lot 7.1 The steel shall conform to the requirements as to 2 in. [50.8 mm] and over in outside diameter not more than 50 tubeschemical composition prescribed in Table 1. and 0.200 in. [5.1 mm] and over in wall thickness 7.2 When Grades 1 or 6 are ordered under this speciﬁcation, Under 2 in. [50.8 mm] but over 1 in. [25.4 not more than 75 tubessupplying an alloy grade that speciﬁcally requires the addition mm] in outside diameter, or over 1 in.of any element other than those listed for the ordered grade in [25.4 mm] in outside diameter and under 0.200 in. [5.1 mm] in thicknessTable 1 is not permitted. However, the addition of elements 1 in. [25.4 mm] or under in outside diameter not more than 125 tubesrequired for the deoxidation of the steel is permitted. 2
A 334/A 334M – 04afurnace, a lot shall include all tubes of the same size and heat, TABLE 4 Maximum Hardness Numberheat treated in the same furnace at the same temperature, time Grade Rockwell Brinellat heat and furnace speed. 1 B 85 16310. Tensile Requirements 3 B 90 190 6 B 90 190 10.1 The material shall conform to the requirements as to 7 B 90 190tensile properties prescribed in Table 3. 8 ... ... 11 B 90 19011. Hardness Requirements 11.1 The tubes shall have a hardness number not exceedingthose prescribed in Table 4. specimens for the welded joint in welded pipe with wall thicknesses of 0.120 in. [3 mm] and larger, when tested at12. Impact Requirements temperatures in conformance with 14.1 shall be not less than 12.1 For Grades 1, 3, 6, 7 and 9, the notched-bar impact the values prescribed in Table 5. The impact test is not requiredproperties of each set of three impact specimens, including for Grade 11. TABLE 3 Tensile Requirements Grade 1 Grade 3 Grade 6 Grade 7 Grade 8 Grade 9 Grade 11 ksi MPa ksi MPa ksi MPa ksi MPa ksi MPa ksi MPa ksi MPaTensile Strength, min 55 380 65 450 60 415 65 450 100 690 63 435 65 450Yield Strength, min 30 205 35 240 35 240 35 240 75 520 46 315 35 240Elongation in 2 in. or 50 mm (or 4D), min, %:Basic minimum elongation for walls 35 30 30 30 22 28 18A 5 / 16 in. [8 mm] and over in thickness, strip tests, and for all small sizes tested in full sectionWhen standard round 2-in. or 50 28 22 22 22 16 ... ... mm gage length or proportionally smaller size specimen with the gage length equal to 4D (4 times the diameter) is usedFor strip tests, a deduction for each 1.75B 1.50B 1.50B 1.50B 1.25B 1.50B ... 1 / 32 in. [0.8 mm] decrease in wall thickness below 5 / 16 in. [8 mm] from the basic minimum elonga- tion of the following percentage points A Elongation of Grade 11 is for all walls and for small sizes tested in full section. B The following table gives the calculated minimum values: Wall Thickness Elongation in 2 in. or 50 mm, min %A in. mm Grade 1 Grade 3 Grade 6 Grade 7 Grade 8 Grade 9 5 / 16 (0.312) 8 35 30 30 30 22 28 9 / 32 (0.281) 7.2 33 28 28 28 21 26 1/4 (0.250) 6.4 32 27 27 27 20 25 7 / 32 (0.219) 5.6 30 26 26 26 18 24 3 / 16 (0.188) 4.8 28 24 24 24 17 22 5 / 32 (0.156) 4 26 22 22 22 16 20 1/8 (0.125) 3.2 25 21 21 21 15 19 3 / 32 (0.094) 2.4 23 20 20 20 13 18 1 / 16 (0.062) 1.6 21 18 18 18 12 16 A Calculated elongation requirements shall be rounded to the nearest whole number. Note—The above table gives the computed minimum elongation values for each 1 / 32 -in. [0.8-mm] decrease in wall thickness. Where the wall thickness lies betweentwo values shown above, the minimum elongation value is determined by the following equations: Grade EquationA 1 E = 56t + 17.50 [E = 2.19t + 17.50] 3 E = 48t + 15.00 [E = 1.87t + 15.00] 6 E = 48t + 15.00 [E = 1.87t + 15.00] 7 E = 48t + 15.00 [E = 1.87t + 15.00] 8 E = 40t + 9.50 [E = 1.56t + 9.50] 9 E = 48t + 13.00 [E = 1.87t + 13.00] A where:E = elongation in 2 in. or 50 mm, %, andt = actual thickness of specimen, in. [mm]. 3
A 334/A 334M – 04a TABLE 5 Impact Requirements for Grades 1, 3, 6, 7, and 9 represented in a heat-treatment load on specimens taken from the ﬁnished tube. This test shall represent only tubes from the Size of Minimum Average Notched Minimum Notched Bar ImpactSpecimen, mm Bar Impact Value of Each Set Value of One Specimen Only same heat, which have wall thicknesses not exceeding by more of Three SpecimensA of a SetA than 1 / 4 in. [6.3 mm] the wall thicknesses of the tube from ft·lbf J ft·lbf J which the test specimens are taken. If heat treatment is10 by 10 13 18 10 14 performed in continuous or batch-type furnaces controlled10 by 7.5 10 14 8 11 within a 50 °F [30 °C] range and equipped with recording10 by 6.67 9 12 7 9 pyrometers which yield complete heat-treatment records, then10 by 5 7 9 5 710 by 3.33 5 7 3 4 one test from each heat in a continuous run only shall be10 by 2.5 4 5 3 4 required instead of one test from each heat in each heat- A Straight line interpolation for intermediate values is permitted. treatment load. 13.8 Impact Tests (Welded Tubes)—On welded tube, addi- tional impact tests of the same number as required in 13.7 shall 12.1.1 If the impact value of one specimen is below the be made to test the weld.minimum value, or the impact values of two specimens are less 13.9 Specimens showing defects while being machined orthan the minimum average value but not below the minimum prior to testing may be discarded and replacements shall bevalue permitted on a single specimen, a retest shall be allowed. considered as original specimens.The retest shall consist of breaking three additional specimensand each specimen must equal or exceed the required average 14. Specimens for Impact Testvalue. When an erratic result is caused by a defective speci- 14.1 Notched-bar impact specimens shall be of the simplemen, or there is uncertainty in test procedures, a retest will be beam, Charpy-type, in accordance with Test Methods E 23,allowed. Type A, with a V notch. Standard specimens 10 by 10 mm in 12.2 For Grade 8 each of the notched bar impact specimens cross section shall be used unless the material to be tested is ofshall display a lateral expansion opposite the notch not less insufficient thickness, in which case the largest obtainablethan 0.015 in. [0.38 mm]. subsize specimens shall be used. Charpy specimens of width 12.2.1 When the average lateral expansion value for the along the notch larger than 0.394 in. [10 mm] or smaller thanthree impact specimens equals or exceeds 0.015 in. [0.38 mm] 0.099 in. [2.5 mm] are not provided for in this speciﬁcation.and the value for one specimen is below 0.015 in. [0.38 mm] 14.2 Test specimens shall be obtained so that the longitudi-but not below 0.010 in. [0.25 mm], a retest of three additional nal axis of the specimen is parallel to the longitudinal axis ofspecimens may be made. The lateral expansion of each of the the tube while the axis of the notch shall be perpendicular toretest specimens must equal or exceed 0.015 in. [0.38 mm]. the surface. On wall thicknesses of 1 in. [25 mm] or less, the 12.2.2 Lateral expansion values shall be determined in specimens shall be obtained with their axial plane located at theaccordance with Test Methods and Deﬁnitions A 370. midpoint; on wall thicknesses over 1 in. [25 mm], the speci- 12.2.3 The values of absorbed energy in foot-pounds and mens shall be obtained with their axial plane located 1⁄2 in.the fracture appearance in percentage shear shall be recorded [12.5 mm] from the outer surface.for information. A record of these values shall be retained for 14.3 When testing welds the specimen shall be, whenevera period of at least 2 years. diameter and thickness permits, transverse to the longitudinal axis of the tube with the notch of the specimen in the welded13. Mechanical Tests joint and perpendicular to the surface. When diameter and 13.1 Tension Test—One tension test shall be made on a thickness does not permit obtaining transverse specimens,specimen for lots of not more than 50 tubes. Tension tests shall longitudinal specimens in accordance with 14.2 shall bebe made on specimens from two tubes for lots of more than 50 obtained. The bottom of the notch shall be located at the weldtubes. joint. 13.2 Flattening Test—One ﬂattening test shall be made onspecimens from each end of one ﬁnished tube of each lot but 15. Impact Testnot the one used for the ﬂare or ﬂange test. 15.1 Except when the size of the ﬁnished tube is insufficient 13.3 Flare Test (Seamless Tubes)—One ﬂare test shall be to permit obtaining subsize impact specimens, all materialmade on specimens from each end of one ﬁnished tube of each furnished under this speciﬁcation and marked in accordancelot, but not the one used for the ﬂattening test. with Section 17 shall be tested for impact resistance at the 13.4 Flange Test (Welded Tubes)—One ﬂange test shall be temperature for the respective grades as prescribed in Table 6.made on specimens from each end of one ﬁnished tube of each 15.1.1 Special impact tests on individual lots of materiallot, but not the one used for the ﬂattening test. may be made at other temperatures if agreed upon between the 13.5 Reverse Flattening Test—For welded tubes, one re- manufacturer and the purchaser.verse ﬂattening test shall be made on a specimen from each 15.2 The notched-bar impact test shall be made in accor-1500 ft [460 m] of ﬁnished tubing. dance with the procedure for the simple beam, Charpy-type of 13.6 Hardness Test—Brinell or Rockwell hardness tests test of Test Methods E 23.shall be made on specimens from two tubes from each lot. 15.3 Impact tests speciﬁed for temperatures lower than +70 13.7 Impact Tests—One notched-bar impact test, consisting °F [20 °C] should be made with the following precautions. Theof breaking three specimens, shall be made from each heat impact test specimens as well as the handling tongs shall be 4
A 334/A 334M – 04a TABLE 6 Impact Temperature TABLE 7 Impact Temperature Reduction Grade Impact Test Temperature Specimen Width Along Notch or Actual Temperature Reduction, Material ThicknessA Degrees Colder °F °C Inches Millimetres °F °C 1 −50 −45 3 −150 −100 0.394 10 (standard size) 0 0 6 −50 −45 0.354 9 0 0 7 −100 −75 0.315 8 0 0 8 −320 −195 0.295 7.5 ( 3 / 4 standard size) 5 3 9 −100 −75 0.276 7 8 4 0.262 6.67 ( 2 / 3 standard size) 10 5 0.236 6 15 8 0.197 5 ( 1 / 2 standard size) 20 11cooled a sufficient time in a suitable container so that both 0.158 4 30 17reach the desired temperature. The temperature shall be mea- 0.131 3.33 ( 1 / 3 standard size) 35 19 0.118 3 40 22sured with thermocouples, thermometers, or any other suitable 0.099 2.5 ( 1 / 4 standard size) 50 28devices and shall be controlled within 63 °F [2 °C]. The A Straight line interpolation for intermediate values is permitted.specimens shall be quickly transferred from the cooling deviceto the anvil of the Charpy impact testing machine and brokenwith a time lapse of not more than 5 s. cation A 1016/A 1016M. The type of test to be used shall be at 15.4 When subsize Charpy impact specimens are used and the option of the manufacturer, unless otherwise speciﬁed inthe width along the notch is less than 80 % of the actual wall the purchase order.thickness of the original material, the speciﬁed Charpy impacttest temperature for Grades 1, 3, 6, 7, and 9 shall be lower than 17. Product Markingthe minimum temperature shown in Table 6 for the respective 17.1 Except as modiﬁed in 16.1.1, in addition to thegrade. Under these circumstances the temperature reduction marking prescribed in Speciﬁcation A 1016/A 1016M, thevalues shall be by an amount equal to the difference (as shown marking shall include whether hot-ﬁnished, cold-drawn, seam-in Table 7) between the temperature reduction corresponding to less, or welded, and the letters “LT” followed by the tempera-the actual material thickness and the temperature reduction ture at which the impact tests were made, except when a lowercorresponding to Charpy specimen width actually tested. The test temperature is required because of reduced specimen size,appendix shows some examples of how the temperature in which case, the higher impact test temperature applicable toreductions are determined. a full-size specimen should be marked. 17.1.1 When the size of the ﬁnished tube is insufficient to16. Hydrostatic or Nondestructive Electric Test obtain subsize impact specimens, the marking shall not include 16.1 Each tube shall be subjected to the nondestructive the letters LT followed by an indicated test temperature unlesselectric test or the hydrostatic test in accordance with Speciﬁ- Supplementary Requirement S 1 is speciﬁed. SUPPLEMENTARY REQUIREMENTS The following supplementary requirement shall apply only when speciﬁed by the purchaser in the inquiry, contract, or order.S1. Nonstandard Test Specimens S1.1 When the size of the ﬁnished tube is insufficient topermit obtaining subsize impact specimens, testing shall be amatter of agreement between the manufacturer and thepurchaser. 5
A 334/A 334M – 04a APPENDIX (Nonmandatory Information) X1. DETERMINATION OF TEMPERATURE REDUCTIONS X1.1 Under the circumstances stated in 15.4, the impact required reduction in test temperature is computed by takingtest temperatures speciﬁed in Table 6 must be lowered. The the difference between the temperature reduction values shownfollowing examples are offered to describe the application of in Table 7 for the actual pipe thickness and the specimen widththe provisions of 15.4. used. X1.1.1 When subsize specimens are used (see 14.1) and the X126.96.36.199 For example, if the pipe were 0.262 in. [6.67 mm]width along the notch of the subsize specimen is 80% or thick and the width along the Charpy specimen notch was 3.33greater of the actual wall thickness of the original material, the mm (1/3 standard size), the test temperature would have to beprovisions of 15.4 do not apply. lowered by 25 °F [14 °C] (that is, the temperature reduction X188.8.131.52 For example, if the actual wall thickness of pipe corresponding to the subsize specimen is 35 °F [19 °C], thewas 0.200 in. [5.0 mm] and the width along the notch of the temperature reduction corresponding to the actual pipe thick-largest subsize specimen obtainable is 0.160 in. [4 mm] or ness is 10 °F [5 °C]; the difference between these two values isgreater, no reduction in test temperature is required. the required reduction in test temperature). X1.1.2 When the width along the subsize specimen notch isless than 80 % of the actual wall thickness of the pipe, the SUMMARY OF CHANGES Committee A01 has identiﬁed the location of selected changes to this speciﬁcation since the last issue, A 334/A 334M – 04, that may impact the use of this speciﬁcation. (Approved May 1, 2004)(1) Moved Notes 2 and 3 into new Section 9 deﬁning the (2) Renumbered subsequent sections and deleted all referencessampling requirements. to Notes 2 and 3 throughout. Committee A01 has identiﬁed the location of selected changes to this speciﬁcation since the last issue, A 334/A 334M – 99, that may impact the use of this speciﬁcation. (Approved March 1, 2004)(1) Replaced Speciﬁcation A 450/A 450M with SpeciﬁcationA 1016/A 1016M in sections 2, 3, 4, 15, and 16. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or email@example.com (e-mail); or through the ASTM website (www.astm.org). 6